2D damping predictions of fiber composite plates: Layup effects


 Brittany Webster
 1 years ago
 Views:
Transcription
1 Available online at Composites Science and Technology 68 (2008) COMPOSITES SCIENCE AND TECHNOLOGY 2D damping predictions of fiber composite plates: Layup effects E.K. Billups, M.N. Cavalli * University of North Dakota, Department of Mechanical Engineering, Stop 8359, 243 Centennial Drive, Grand Forks, ND , United States Received 29 November 2006; received in revised form 25 May 2007; accepted 12 September 2007 Available online 20 September 2007 Abstract Several twodimensional theories for predicting the specific damping capacity (SDC) of fiber composite laminates are compared. The theories considered are those of Adams and Bacon, Adams and Maheri, Ni and Adams and Saravanos and Chamis. No interlaminar effects are considered. Results show that the theory of Saravanos and Chamis provides the most consistent fit to experimental results for a range of material properties and laminate layups. For some laminates, however, the Saravanos and Chamis method seems to predict the wrong trend in SDC variation versus layup angle. It is not clear from the current work whether this result is due to the absence of interlaminar effects in the theory or the presence of a threedimensional stress state in the laminate. Ó 2007 Elsevier Ltd. All rights reserved. Keywords: A. Polymer matrix composites; A. Structural materials; B. Modeling; C. Laminate theory 1. Introduction Energy dissipation, or damping, is an important consideration in a variety of engineering designs. Composite materials offer the unique ability to tailor damping behavior, and other properties, for specific applications [1 4]. As a result, composites can be desirable choices in applications as varied as wind turbine blades [5 9], beams and shafts [10,11] and control surfaces [12,13]. A full analysis of damping performance for arbitrary composite structures typically requires threedimensional numerical analysis due to the mathematical complexity of the problem [14 17]. Simplified, twodimensional analyses based on the principles of Classical Laminate Theory (CLT) have shown good agreement for particular materials, layups, and geometries, however [1 4,18]. The goal of the current work is to compare several theories available in the literature for predicting the specific damping capacity (SDC) of composite laminates. Theories of Adams and Bacon [1], Ni and Adams [3], Adams and * Corresponding author. Tel.: ; fax.: address: (M.N. Cavalli). Maheri [18] and Saravanos and Chamis [19,20] will be examined. Results from each theory will be compared with experimental measurements of SDC values. These comparisons will help illustrate the strengths and shortcomings of each theory as well as the use of twodimensional damping predictions generally. An example will then be presented of how the Saravanos and Chamis method can be applied to a composite beam whose plies are assembled at arbitrary angles. Damping, stiffness and deflection predictions for this arbitrary laminate will be presented graphically in several forms, each with specific advantages in terms of selecting a layup for a particular set of design requirements. This example will illustrate the usefulness of the technique in designing fiber composite structures. 2. Theory 2.1. Overview All theories compared in this work are based on the assumptions of classical laminate theory for orthotropic materials [21,22]. In short, this implies perfect bonding between plies, no out of plane stresses or strains and small, /$  see front matter Ó 2007 Elsevier Ltd. All rights reserved. doi: /j.compscitech
2 728 E.K. Billups, M.N. Cavalli / Composites Science and Technology 68 (2008) elastic deformations [21,22]. Matrices of applied forces and moments are written as [N] and [M], respectively, with subscripts used to indicate specific components. The typical notation used in this paper for subscripts, unless otherwise noted, is number subscripts, i.e. 1, 2, or 12, are used to denote principal material directions of a lamina while letter subscripts, i.e. x, y, orxy, denote the global coordinates of the laminate. The two coordinate systems are typically offset by an angle, h. For elastic deformations, the strain energy stored in each ply can be separated into three components: strain energy in the fiber direction, strain energy transverse to the fiber direction, and strain energy in shear. Some amount of each of these components is dissipated during deformation. One way to quantify this dissipation is by using the specific damping capacity which is defined as the strain energy dissipated during a stress cycle, DU, divided by the maximum strain energy during a stress cycle, Eq. (1). w ¼ DU ð1þ U max The total strain energy dissipated for each lamina is the product of the lamina strain energy components with the damping coefficient for the appropriate mode of deformation, all integrated over the thickness of the ply. Consequently, this method requires knowledge of three damping coefficients for each lamina: the longitudinal (fiber direction) coefficient, w Lk, the transverse coefficient, w Tk, and the inplane shear coefficient, w LTk, where the subscript k denotes these are the properties of the kth lamina. The damping coefficients can be determined via tests on unidirectional laminates under various angles of loading. The energy dissipation can be summed over the total number of plies and, using the total energy dissipated in the laminate, the overall specific damping capacity (SDC) written as [1]: w laminate ¼ w 1 þ w 2 þ w 12 ð2þ 2.2. Adams and Bacon theory Adams and Bacon [1] presented a general equation to predict the SDC of beams for applied forces, {N}, and moments, {M}. The equation can be used for any laminate configuration and the lamina damping coefficients (w Lk, w Tk, w LTk ) are allowed to be stress dependent: w laminate ¼ 2P n R hk h k 1 ðdðdu 1 ÞþdðDU 2 ÞþdðDU 12 ÞÞdz fng T fe o gþfmg T fjg ð3þ Eq. (3) includes contributions from all inplane stresses but does not allow for outofplane contributions to energy dissipation. The latter limitation is consistent for all theories presented in this paper. The number of terms involved in Eq. (3) leads to a level of complexity that can typically only be handled using numerical techniques. Adams and Bacon recognized this and derived several approximations to Eq. (3) that lend themselves to easier solutions by neglecting certain stresses and strains or limiting the allowable layups [1] Ni and Adams theory Additional damping prediction equations were developed by Ni and Adams [3]. They assumed free flexure deformation, stressindependent damping coefficients and a symmetric layup [3]. This final assumption leads to no midplane strains under classical laminate plate theory. In addition to neglecting r y and s xy, Ni and Adams also argued that the transverse strain, e y, in each lamina will be much smaller than the longitudinal and shear strains and could be neglected [3], resulting in Eqs. (4) (6) w 1 ¼ 8w X p=2 L m 2 ðq k C 11 p 3 11 C 11 þ Q k 12 C 12 þ Q k 16 C 16Þ ðm 2 C 11 þ mnc 16 ÞW k ð4þ w 2 ¼ 8w X p=2 T n 2 ðq k C 11 p 3 11 C 11 þ Q k 12 C 12 þ Q k 16 C 16Þ ðn 2 C 11 mnc 16 ÞW k ð5þ w 12 ¼ 8w X p=2 LT mnðq k C 11 p 3 11 C 11 þ Q k 12 C 12 þ Q k 16 C 16Þ ð2mnc 11 m 2 n 2 C16 ÞW k ð6þ where [C] is the normalized flexural compliance of the laminate, [Q k ] is the stiffness of the kth lamina, p is the total number of plies present in the laminate and W k is a weighting factor based on the position of the kth lamina within the laminate [3] Adams and Maheri theory Revisions to the Ni and Adams equations were made by Adams and Maheri [18]. The derivation of the equation deviated from the method used by Ni and Adams but the final result is similar. In short, the Adams and Maheri theory is the Ni and Adams theory with slight notational changes and the transverse lamina strain, e y, term included [18] Saravanos and Chamis theory The expression for the strain energy of a general laminate under general loading has been formulated by Tse and Lai [23] and Saravanos and Chamis [19]. Saravanos and Chamis have also written the three SDC components in matrix form [19,20]. These results can be combined to give an expression for the SDC of an arbitrary laminate under general loading which can be written as
3 E.K. Billups, M.N. Cavalli / Composites Science and Technology 68 (2008) T N A B T A D B D A B N M C D B w laminate ¼ D D D C D M T N A B T ð7þ N M C D M where A *, B *, C * and D * represent the components of the inverse of the original material stiffness matrix [21,22]. A D, B D, C D and D D are the components of the original stiffness matrix multiplied by appropriate damping coefficients. Eq. (7) is the basis of the Saravanos and Chamis theory. It should be noted that in their original work, Saravanos and Chamis also include the possibility of interlaminar effects, but those are not considered here [21,22]. Though it is not perhaps immediately apparent, the form of the Saravanos and Chamis theory expression for laminate damping is very similar in form to that previously developed by Adams and Bacon (Eq. (3)). An important distinction is that Eq. (7) is written in terms of stiffnesses and strains while Eq. (3) is written in terms of stresses and compliances. This made sense for Adams and Bacon because they included stressdependence in their damping coefficients which the Saravanos and Chamis theory does not. The tradeoff, however, is that the Adams and Bacon form is less computationally efficient. 3. Results and discussion 3.1. Comparison with previous work Experimentally determined values for the specific damping coefficients were obtained from the literature for several variations of Eglass epoxy and carbon epoxy fiber composites under freefree flexural loading [1 3]. Table 1 lists the material properties for each laminate [1 3]. These values were used in the Ni and Adams [3], Adams and Maheri [2] and Saravanos and Chamis [19] theories to calculate the predicted values of SDC for various fiber geometries. All calculations were performed using MATLAB (The Mathworks, Natick, MA). Unfortunately, the general theory of Adams and Bacon can only be compared with the data presented in the original paper [1]. This is because the theory allows for stress dependent damping coefficients but does not explicitly identify the relationship between the coefficients and the lamina stresses. The results of Adams and Bacon could thus not be recalculated for other laminate geometries. Transcription of data points from the original plots has been used to recreate their curves in the current work. Adams and Maheri [2] measured the specific damping capacity of two laminate configurations of Fibredux 913/ glass fiber composites. The first was a balanced symmetric angleply laminate, [ h /+h / h /+h ] s and the second was a symmetric unidirectional laminate, [h ] 8. Beams were cut from plates with the above layups and excited at the fundamental flexural mode of vibration. The variation of the SDC with fiber orientation for these configurations is shown in Figs. 1 and 2, respectively. Note that results from two beam widths are plotted in Fig. 1. No experimental uncertainty is presented with the original data, but the beam width does not appear to cause a dramatic effect on the damping [2]. Results from Kyriazoglou and Guild indicate this may not be the case for larger ranges of aspect ratios [24]. All theories predict the SDC values reasonably well for both laminates. The blank legend symbol for the Adams/Maheri theory indicates that this theory is identical to the theory listed above it (Saravanos, in this case) for this particular laminate. Figs. 3 and 4 show results from experiments conducted by Adams and Bacon [1] on DX209/carbon fiber composite laminates. The layup in Fig. 3 is [h] 10 and the layup in Fig. 4 is [+h/ h] 5. No information is given regarding the difference between experimental data sets 1 and 2 in Fig. 3 [1]. The Sarvanos and Chamis theory and the Adams and Bacon theory provide the most consistent fit in terms of both magnitude of the predicted SDC and shapes of the curves. Fig. 4 shows that there are some layup/material Table 1 Material properties for damping results presented. Material E 1 (ksi GPa) E 2 (ksi GPa) G 12 (ksi GPa) m 12 w L (%) w T (%) w LT (%) V f References Fiber Matrix Eglass Epoxy (DX 210) [3] Eglass Epoxy (Fibredux 913) [2] HMS carbon Epoxy (DX 209) 27, [1] HMS carbon Epoxy (DX 210) 25, [3]
4 730 E.K. Billups, M.N. Cavalli / Composites Science and Technology 68 (2008) Fig. 1. Variation of the specific damping capacity with fiber orientation for a glass/epoxy (Fiberdux 913G) laminate with a symmetric angleply layup of [ h /+h / h /+h ] s. Fig. 4. Variation of the specific damping capacity with fiber orientation for carbon/epoxy (HMS/DX209) laminate with a angle ply layup of [+h / h ] 5. Fig. 2. Variation of the specific damping capacity with fiber orientation for a glass/epoxy (Fiberdux 913G) laminate with a unidirectional layup of [h ] 8.. combinations where the 2D theories are not able to fully predict the behavior of the material. This may be due to interlaminar effects or may indicate that a threedimensional stress state exists for this laminate. Since no uncertainty is quoted on the experimental data, however, no firm conclusion can be reached. Ni and Adams [3] investigated symmetric laminates, [h /(h + 90) /(h + 45) /(h 45) ] s, for both glass and carbon fibers with DX210 epoxy. The widthtolength ratios of the beams used in the experimental damping determination was 1:17. The variation of the SDC with respect to the outer ply orientation for a glass and carbons composites is shown in Figs. 5 and 6, respectively. The damping trend is captured reasonably well by all theories for the glass fiber composite but significant discrepancies are apparent for the carbon fiber material. Both the Adams and Maheri and Ni and Adams theories significantly overpredict the damping for positive angles and neither capture the shape of the SDC curve for positive Fig. 3. Variation of the specific damping capacity with fiber orientation for carbon/epoxy (HMS/DX209) laminate with a unidirectional layup of [h ] 10. Fig. 5. Variation of the specific damping capacity with outer ply fiber orientation for a glass/epoxy (glass/dx210) laminate with a layup of [h / (h + 90) /(h + 45) /(h 45) ] s.
5 E.K. Billups, M.N. Cavalli / Composites Science and Technology 68 (2008) of w 2 are positive for all orientations in the Ni and Adams and Saravanos and Chamis theories but the shapes of the two curves are significantly different. These differences can be traced back to the fundamentally different assumptions regarding stresses and strains within the plies Predictions of damping for arbitrary laminates Fig. 6. Variation of the specific damping capacity with outer ply fiber orientation for a carbon/epoxy (HMS/DX210) laminate with a layup of [h /(h + 90) /(h + 45) /(h 45) ] s. values of h as well as the Saravanos and Chamis theory. For negative values of h, both Adams and Maheri and Ni and Adams again overpredict the measured damping. The Saravanos and Chamis theory gives reasonable predictions for the SDC magnitude at negative values of h, but seems to predict the wrong shape for the SDC curve near h ¼ 45. It is not clear if the discrepancies between the theory and data for this laminate arise from uncertainty in the experimental results, edge effects, interlaminar effects or a threedimensional stress state. Fig. 7 shows an interesting result for the Adams and Maheri theory applied to the [h /(h + 90) /(h + 45) / (h 45) ] s carbon/dx210 laminate. The w 2 component of the SDC is plotted versus outer ply orientation. For some orientations, the Adams and Maheri theory actually predicts negative values of w 2, an unrealistic result that implies energy generation, rather than damping. Values The Saravanos and Chamis theory will now be applied to an arbitrary laminate to illustrate the information that can be provided regarding composite laminate properties. Values from Table 1 for the Ni and Adams Fibredux 913/glass fiber damping coefficients will be used for all predictions [3]. The laminate to be analyzed is of the form [h 1 / (h 1 + a) /(h 1 a) /(h 1 + a) / (h 1 a) / (h 2 a) / (h 2 + a) / (h 2 a) / (h 2 + a) / h 2 ], where h 1, h 2, and a could take on any value from 0 to 180. First, let us select a single value for the offset angle, a ¼ 90. Fig. 8 illustrates how the SDC of the resulting laminate varies with changes in h 1 and h 2 under M x loading. The maximum possible value of SDC is approximately 5.7% and occurs when h 1 ¼ 48 and h 1 ¼ 132. Note that the resolution of Fig. 8 for both h 1 and h 2 is 2. The minimum level of damping that can be achieved in this laminate is about 1.7%, when h 1 ¼ h 2 ¼ 90. Referring to Table 1, most energy in this material is dissipated by deformations in the matrix, so both of these results make sense. Values of h 1 and h 2 near 45 result in a large contribution from matrix deformation and lead to large overall values of energy dissipation. In contrast, values of h 1 and h 2 near 90 result in most of the laminate (8 of 10 plies) having Fig. 7. Variation of the specific damping capacity component w 2 with outer ply fiber orientation for a carbon/epoxy (HMS/DX210) laminate with a layup of [h /(h + 90) /(h + 45) /(h 45) ] s. Fig. 8. Variation of SDC (%) prediction with fiber orientation angle for glass/epoxy in a symmetric layup of [h 1 /(h ) /(h 1 90) /(h ) / (h 1 90) /(h 2 90) /(h ) /(h 2 90) /(h ) /h 2 ] for M x 5 0.
6 732 E.K. Billups, M.N. Cavalli / Composites Science and Technology 68 (2008) Fig. 9. Variation of SDC (%) prediction with fiber orientation angle for glass/epoxy in a symmetric layup of [h 1 /(h ) /(h 1 90) /(h ) / (h 1 90) ] s for M x 5 0. the fiber direction aligned along the xaxis. This leads to very little damping contribution from matrix deformations and minimizes the overall energy dissipation. It is necessary to recognize that the value of the SDC may not be the only laminate property of interest. If a laminate deforms in an undesirable way during loading or curing (e.g. warps), it may not be able to fulfill its design requirements despite desirable energy dissipation characteristics. Similarly, the laminate must possess the proper effective stiffness under a given mode of loading. Contours showing laminate effective stiffness and warpage behavior as a function of layup geometry can be created easily by incorporating the appropriate equations into the MATLAB code. These can then be compared with the SDClayup contour (Fig. 8) to optimize the composite layup. It is possible that the entire design space of Fig. 8 is not attainable or desirable in a given manufacturing situation. The simplicity of a symmetric layup may be desirable, for example. In such a situation, a second method of analyzing the Saravanos and Chamis theory results would be to pull out SDC values along a specified section of Fig. 8. For a symmetric laminate, Fig. 9 is the result. Fig. 9 indicates that values of h 1 must be between 31 and 59 to achieve damping within about 10% of the maximum value for a symmetric laminate. To be within about 10% of the minimum value, h 1 must be between 85 and 95. Corresponding sections could be constructed for various conditions (h 1 ¼ constant, h 2 ¼ constant, h 1 / h 2 ¼ constant, etc.). A third method of using the Saravanos and Chamis technique is to allow all angles, h 1, h 2, and a, to vary from 0 to 180. This method allows the full range of laminate properties that can be achieved to be identified. Fig. 10 shows the range of SDC that are predicted for this laminate as a function of the effective flexural stiffness. The maximum achievable value of SDC is approximately 6% and occurs in a laminate with h 1 ¼ h 2 ¼ 48 and a ¼ 0. Minimum damping (0.8%) occurs in a laminate with h 1 ¼ h 2 ¼ a ¼ 0. The fact that the maximum damping is Fig. 10. SDC flexural modulus envelope showing all possible combinations predicted by CLT theory for glass/epoxy laminate with layup [h 1 /(h 1 + h) /(h 1 h) /(h 1 + h) /(h 1 h) /(h 2 h) /(h 2 + h) /(h 2 h) / (h 2 + h) /h 2 ]. in a layup of approximately ±45 and the minimum damping is in the stiffest laminates is not surprising given the material properties. What makes Fig. 10 interesting is the fact that it clearly shows that for a given value of effective stiffness, it may be possible to tailor the SDC of the laminate over a relatively large range. Similar design envelopes can be defined for other types of loadings as well as laminate outofplane deformations. The calculations required to construct Fig. 10 resulted in approximately 26,000 data points and required approximately 45 minutes to complete on a 3GHz Pentium 4 PC. With the information from the CLT method presented in this form, damping, stiffness and warpage of potential laminates can be quickly assessed. 4. Conclusions A comparison of the damping predictions from several twodimensional composite laminate theories has been conducted. Results indicate that the general theory of Saravanos and Chamis most consistently agrees with experimental results. Certain layup/material combinations show significant deviations between theoretical predictions and experimental data, particularly with stiffer carbon reinforcement. More work is needed to determine whether these differences arise from interlaminar, edge or threedimensional stress effects. The Saranavos and Chamis method has been used to predict the damping, stiffness and outofplane deformation for an arbitrary composite laminate. Several approaches to the analysis are presented to quickly identify the performance envelope of a specific laminate and to tailor properties such as the specific damping coefficient (SDC) and the effective stiffness. These approaches could be applied to structures such as wind turbine blades where energy dissipation and stiffness both play a large role in successful design performance.
7 E.K. Billups, M.N. Cavalli / Composites Science and Technology 68 (2008) Acknowledgement Financial support of Mr. Billups from the UND Mechanical Engineering Department during the course of this work is gratefully acknowledged. References [1] Adams RD, Bacon DGC. Effect of fibre orientation and laminate geometry on the dynamic properties of CFRP. J Compos Mater 1973;7: [2] Adams RD, Maheri MR. Dynamic flexural properties of anisotropic fibrous composite beams. Compos Sci Technol 1994;50(4): [3] Ni RG, Adams RD. The damping and dynamic moduli of symmetric laminated composite beams theoretical and experimental results. J Compos Mater 1984;18(2): [4] Chandra R, Singh SP, Gupta K. Damping studies in fiberreinforced composites a review. Compos Struct 1999;46: [5] Bechly ME, Clausen PD. Structural design of a composite wind turbine blade using finite element analysis. Comput Struct 1999;63(3): [6] Lobitz D, Veers PS, Migliore PG. Enhanced performance of HAWTs using adaptive blades. In: Proceedings of the wind 1996 ASME wind energy symposium. Houston, Texas, USA: ASME; [7] Lee AT, Flay RGJ. Compliant blades for wind turbines. The Inst Prof Eng New Zealand 1999;26(1):7 12. [8] Garfinkle M. Twisting smartly in the wind. Aerospace Amer 1994;32(7): [9] Chandra R. Active shape control of composite blades using shape memory actuation. Smart Mater Struct 2000;10(5): [10] Bert CW, Kim C. Whirling of compositematerial driveshafts including bendingtwisting coupling and transverse shear deformation. J Vibr Acoust 1995;117(1): [11] Lentz WK, Armnaios EA. Optimum coupling in thinwalled, closedsection composite beams. J Aerospace Eng 1998;11(3):81 8. [12] Klous H, Mirza S. Piezoelectric induced bending and twisting of laminated composite shallow shells. Smart Mater Struct 2000;9(4): [13] Kim C, Park BS, Goo NS. Shape changes by coupling bending and twisting of shapememoryalloyembedded composite beams. Smart Mater Struct 2002;11(4): [14] Wetherhold RC, Panthalingal N. Piezoelectric PZT/epoxy composites for controlling torsional motion. J Intell Mater Syst Struct 1994;5: [15] Chandra R, Singh SP, Gupta K. A study of damping in fiberreinforced composites. J Sound Vibr 2003;262: [16] Hwang SJ, Gibson RF. The effects of threedimensional states of stress on damping in laminated composites. Compos Sci Technol 1991;41: [17] Hwang SJ, Gibson RF. Influence of bendingtwisting and extensionbending coupling on damping of laminated composites. J Mater Sci 1993;28:1 8. [18] Adams RD, Maheri MR. Damping in advanced polymer matrix composites. J Alloys Comp 2003;355(1 2): [19] Saravanos DA, Chamis CC. Unified micromechanics of damping for unidirectional fiber reinforced composites, NASA TM National Aeronautics and Space Administration, Cleveland; [20] Saravanos DA, Chamis CC, Mechanics of damping for fiber composite laminates including hygrothermal effects, NASA TM National Aeronautics and Space Administration, Cleveland; [21] Jones RM. Mechanics of composite materials. Philadelphia: Taylor & Francis; [22] Kaw AK. Mechanics of composite materials. Boca Raton, Florida: CRC Press; [23] Tse PC, Lai TC. Expression for the strain energy of laminated composite thin shells. Int J Mech Eng Educ 1995;23(2): [24] Kyriazoglou C, Guild FJ. Finite element prediction of damping of composite GFRP and CFRP laminates a hybrid formulation vibration damping experiments and Rayleigh damping. Compos Sci Technol 2006;66(3 4):
Passive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of Materials Science and Engineering A 6 () 354 doi:.765/663/6..5 D DAVID PUBLISHING Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K * and V V Subba Rao Faculty
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationHygrothermal stresses in laminates
Hygrothermal stresses in laminates Changing environment conditions (temperature and moisture) have an important effect on the properties which are matrix dominated. Change in temperaturet and moisture
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationPLY LEVEL UNCERTAINTY EFFECTS ON FAILURE OF COMPOSITE
7th European Workshop on Structural Health Monitoring July 811, 2014. La Cité, Nantes, France More Info at Open Access Database www.ndt.net/?id=17206 PLY LEVEL UNCERTAINTY EFFECTS ON FAILURE OF COMPOSITE
More informationModule 5: Laminate Theory Lecture 17: Laminate Constitutive Relations. The Lecture Contains: Laminate Constitutive Relations
Lecture 17: Laminate Constitutive Relations The Lecture Contains: Laminate Constitutive Relations Classification of Laminates CrossPly Laminates Specially Orthotropic Laminates Examples Homework References
More informationAssessment Methods of Mechanical Properties of Composite Materials
Mechanics and Mechanical Engineering Vol. 21, No. 4 (2017) 1005 1018 c Lodz University of Technology Assessment Methods of Mechanical Properties of Composite Materials Monika Kamocka Radoslaw J. Mania
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationDynamic and buckling analysis of FRP portal frames using a lockingfree finite element
Fourth International Conference on FRP Composites in Civil Engineering (CICE8) 2224July 8, Zurich, Switzerland Dynamic and buckling analysis of FRP portal frames using a lockingfree finite element F.
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More informationThermal Vibration of Magnetostrictive Material in Laminated Plates by the GDQ Method
The Open echanics Journal, 007, 1, 937 9 Thermal Vibration of agnetostrictive aterial in Laminated Plates by the GDQ ethod C.C. Hong * Department of echanical Engineering, Hsiuping Institute of Technology,
More informationA HIGHERORDER BEAM THEORY FOR COMPOSITE BOX BEAMS
A HIGHERORDER BEAM THEORY FOR COMPOSITE BOX BEAMS A. Kroker, W. Becker TU Darmstadt, Department of Mechanical Engineering, Chair of Structural Mechanics Hochschulstr. 1, D64289 Darmstadt, Germany kroker@mechanik.tudarmstadt.de,
More informationPresented By: EAS 6939 Aerospace Structural Composites
A Beam Theory for Laminated Composites and Application to Torsion Problems Dr. BhavaniV. Sankar Presented By: Sameer Luthra EAS 6939 Aerospace Structural Composites 1 Introduction Composite beams have
More informationEffect of Thermal Stresses on the Failure Criteria of Fiber Composites
Effect of Thermal Stresses on the Failure Criteria of Fiber Composites Martin Leong * Institute of Mechanical Engineering Aalborg University, Aalborg, Denmark Bhavani V. Sankar Department of Mechanical
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More informationSIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO MULTIPLE LOADING WITH MEMBRANEFLEXION COUPLING EFFECTS
VOL. 5, NO. 4, APRIL 010 ISSN 18196608 006010 Asian Research Publishing Network (ARPN). All rights reserved. SIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO
More informationComparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost
Comparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost 1 Mihir A. Mehta, 2 Satyen D. Ramani 1 PG Student, Department
More informationBending Analysis of Symmetrically Laminated Plates
Leonardo Journal of Sciences ISSN 15830233 Issue 16, JanuaryJune 2010 p. 105116 Bending Analysis of Symmetrically Laminated Plates Bouazza MOKHTAR 1, Hammadi FODIL 2 and Khadir MOSTAPHA 2 1 Department
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationVIBRATION AND DAMPING ANALYSIS OF FIBER REINFORCED COMPOSITE MATERIAL CONICAL SHELLS
VIBRATION AND DAMPING ANALYSIS OF FIBER REINFORCED COMPOSITE MATERIAL CONICAL SHELLS Mechanical Engineering Department, Indian Institute of Technology, New Delhi 110 016, India (Received 22 January 1992,
More informationComposite Structures. Indian Institute of Technology Kanpur
Mechanics of Laminated Composite Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 23 Analysis of an Orthotropic Ply Lecture Overview Introduction Engineering constants for an 2
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationModule 5: Laminate Theory Lecture 19: Hygro thermal Laminate Theory. Introduction: The Lecture Contains: Laminate Theory with Thermal Effects
Module 5: Laminate Theory Lecture 19: Hygro thermal Laminate Theory Introduction: In this lecture we are going to develop the laminate theory with thermal and hygral effects. Then we will develop the
More informationFLEXURAL RESPONSE OF FIBER RENFORCED PLASTIC DECKS USING HIGHERORDER SHEAR DEFORMABLE PLATE THEORY
AsiaPacific Conference on FRP in Structures (APFIS 2007) S.T. Smith (ed) 2007 International Institute for FRP in Construction FLEXURAL RESPONSE OF FIBER RENFORCED PLASTIC DECKS USING HIGHERORDER SHEAR
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 34 Thermal Stresses in Plates Lecture Overview Introduction Mechanical and Thermal Strains
More informationVIBRATION CONTROL OF RECTANGULAR CROSSPLY FRP PLATES USING PZT MATERIALS
Journal of Engineering Science and Technology Vol. 12, No. 12 (217) 33983411 School of Engineering, Taylor s University VIBRATION CONTROL OF RECTANGULAR CROSSPLY FRP PLATES USING PZT MATERIALS DILEEP
More informationS. Srinivasan, Technip Offshore, Inc., Houston, TX
9 th ASCE Specialty Conerence on Probabilistic Mechanics and Structural Reliability PROBABILISTIC FAILURE PREDICTION OF FILAMENTWOUND GLASSFIBER Abstract REINFORCED COMPOSITE TUBES UNDER BIAXIAL LOADING
More informationUNEXPECTED TWISTING CURVATURE GENERATION OF BISTABLE CFRP LAMINATE DUE TO THE UNCERTAINTY OF LAYUP SEQUENCE AND NEGATIVE INITIAL CURVATURE
THE 9 TH INTERNATIONA CONFERENCE ON COMPOSITE MATERIAS UNEXPECTED TWISTING CURVATURE GENERATION OF BISTABE CFRP AMINATE DUE TO THE UNCERTAINTY OF AYUP SEQUENCE AND NEGATIVE INITIA CURVATURE J. Ryu, JG.
More informationOnline publication date: 23 October 2010
This article was downloaded by: [informa internal users] On: 1 November 2010 Access details: Access Details: [subscription number 755239602] Publisher Taylor & Francis Informa Ltd Registered in England
More informationA copy can be downloaded for personal noncommercial research or study, without prior permission or charge
York, C. B. (2015) Influence of bending twisting coupling on compression and shear buckling strength. Stability of Structures 14th Symposium, Zakopane, Poland, 812 Jun 2015. Copyright 2015 The Author.
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationTHE MUTUAL EFFECTS OF SHEAR AND TRANSVERSE DAMAGE IN POLYMERIC COMPOSITES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS THE MUTUAL EFFECTS OF SHEAR AND TRANSVERSE DAMAGE IN POLYMERIC COMPOSITES L.V. Smith 1 *, M. Salavatian 1 1 School of Mechanical and Materials
More informationAuthor manuscript, published in "EWSHM  7th European Workshop on Structural Health Monitoring (2014)" 7th European Workshop on Structural Health Monitoring July 811, 2014. La Cité, Nantes, France CURE
More informationNonlinearities in mechanical behavior of textile composites
Composite Structures 71 (25) 61 67 www.elsevier.com/locate/compstruct Nonlinearities in mechanical behavior of textile composites Enrico DÕAmato Energetics Departement, L Aquila University, 674 Monteluco
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationThe Effect of Fiber Orientation and Laminate Stacking Sequences on the Torsional Natural Frequencies of Laminated Composite Beams
Journal of Mechanical Design and Vibration, 13, Vol. 1, No. 1, 6 Available online at http://pubs.sciepub.com/jmdv/1/1/4 Science and Education Publishing DOI:1.1691/jmdv114 The Effect of Fiber Orientation
More informationModeling and analysis of the electrical resistance measurement of carbon fiber polymer matrix composites
Composites Science and Technology 67 (2007) 2513 2520 COMPOSITES SCIENCE AND TECHNOLOGY www.elsevier.com/locate/compscitech Modeling and analysis of the electrical resistance measurement of carbon fiber
More informationON THE NUMERICAL ANALYSIS OF COMPOSITE MATERIAL
The 4th International Conference Advanced Composite Materials Engineering COMAT 8 October, Brasov, Romania O THE UMERICAL AALYSIS OF COMPOSITE MATERIAL D.D. icoara Transilvania University, City Brasov,
More informationA Study on the Tube of Integral Propeller Shaft for the Rearwheel Drive Automobile Using Carbon Composite Fiber
A Study on the Tube of Integral Propeller Shaft for the Rearwheel Drive Automobile Using Carbon Composite Fiber Kibong Han Mechatronics Department, Jungwon University, 85 Munmuro, Goesangun, South Korea.
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationFREE VIBRATION OF THERMALLY PRE/POSTBUCKLED CIRCULAR THIN PLATES EMBEDDED WITH SHAPE MEMORY ALLOY FIBERS
Journal of Thermal Stresses, 33: 79 96, 2010 Copyright Taylor & Francis Group, LLC ISSN: 01495739 print/1521074x online DOI: 10.1080/01495730903409235 FREE VIBRATION OF THERMALLY PRE/POSTBUCKLED CIRCULAR
More informationDesign of Hybrid Composites for Axial loads with Zero Coefficient of Thermal Expansion
Design of Hybrid Composites for Axial loads with Zero Coefficient of Thermal Expansion Zaffar M. Khan 1 and Asim Shahzad 2 Institute of Space Technology, Islamabad, Pakistan, 44000 Aerospace structures
More informationEXPLICIT DYNAMIC SIMULATION OF DROPWEIGHT LOW VELOCITY IMPACT ON CARBON FIBROUS COMPOSITE PANELS
EXPLICIT DYNAMIC SIMULATION OF DROPWEIGHT LOW VELOCITY IMPACT ON CARBON FIBROUS COMPOSITE PANELS Umar Farooq and Karl Gregory School of Built Environment and Department of Engineering, University of Bolton,
More informationTheoretical Approach to Predict Transverse Impact Response of VariableStiffness Curved Composite Plates
*Manuscript Click here to view linked References 1 1 1 1 1 1 1 0 1 0 1 0 1 0 1 0 1 Theoretical Approach to Predict Transverse Impact Response of VariableStiffness Curved Composite Plates B. Arachchige,
More informationMechanical and Thermal Properties of Coir Fiber Reinforced Epoxy Composites Using a Micromechanical Approach
Mechanical and Thermal Properties of Coir Fiber Reinforced Epoxy Composites Using a Micromechanical Approach Sandhyarani Biswas Department of Mechanical Engineering, N.I.T Rourkela, INDIA Abstract: Nowadays,
More informationFINITE ELEMENT AND EXPERIMENTAL STUDY OF NOVEL CONCEPT OF 3D FIBRE CELL STRUCTURE
FINITE ELEMENT AND EXPERIMENTAL STUDY OF NOVEL CONCEPT OF 3D FIBRE CELL STRUCTURE M. Růžička, V. Kulíšek 2, J. Had, O. Prejzek Department of Mechanics, Biomechanics and Mechatronics, Faculty of Mechanical
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationTESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS
TESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS I. M. Daniel, J. L. Abot, and K. A. Wang Walter P. Murphy Professor, Departments of Civil and Mechanical Engineering, Robert R. McCormick School of Engineering
More informationA coupled field finite element model to predict actuation properties of piezoelectrically actuated bistable composites.
A coupled field finite element model to predict actuation properties of piezoelectrically actuated bistable composites. P.F.Giddings, C.R.Bowen, H.A.Kim University of Bath, UK Dept. Mech. ng, University
More informationThermal deformation compensation of a composite beam using piezoelectric actuators
INSTITUTE OF PHYSICS PUBLISHING Smart Mater. Struct. 13 (24) 3 37 SMART MATERIALS AND STRUCTURES PII: S9641726(4)79738 Thermal deformation compensation of a composite beam using piezoelectric actuators
More informationCHEME2200: Polymer blends and composites Fibre architecture and principles of reinforcement
CHEME2200: Polymer blends and composites Fibre architecture and principles of reinforcement Mark Hughes 19 th September 2016 Outline Fibre architecture Volume fraction and the rule of mixtures Principle
More informationFree Vibration Response of a Multilayer Smart Hybrid Composite Plate with Embedded SMA Wires
11(2014) 279298 Free Vibration Response of a Multilayer Smart Hybrid Composite Plate with Embedded SMA Wires Abstract In this paper, free vibration response of a hybrid composite plate was studied. Effects
More informationThe stiffness tailoring of megawatt wind turbine
IOP Conference Series: Materials Science and Engineering OPEN ACCESS The stiffness tailoring of megawatt wind turbine To cite this article: Z M Li et al 2013 IOP Conf. Ser.: Mater. Sci. Eng. 52 052008
More informationApplication of piezoelectric actuators to active control of composite spherical caps
Smart Mater. Struct. 8 (1999 18. Printed in the UK PII: S964176(9916614 Application of piezoelectric actuators to active control of composite spherical caps Victor Birman, Gareth J Knowles and John J
More informationA synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks
Article A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks JOURNAL OF COMPOSITE MATERIALS Journal of Composite Materials 0(0) 7! The Author(s) 0 Reprints
More informationDynamic Analysis of Laminated Composite Plate Structure with Square CutOut under Hygrothermal Load
Dynamic Analysis of Laminated Composite Plate Structure with Square CutOut under Hygrothermal Load Arun Mukherjee 1, Dr. Sreyashi Das (nee Pal) 2 and Dr. A. Guha Niyogi 3 1 PG student, 2 Asst. Professor,
More informationNUMERICAL FEM ANALYSIS FOR THE PART OF COMPOSITE HELICOPTER ROTOR BLADE
Journal of KONES Powertrain and Transport, Vol. 19, No. 1 2012 NUMERICAL FEM ANALYSIS FOR THE PART OF COMPOSITE HELICOPTER ROTOR BLADE Hubert D bski Lublin University of Technology, Department of Machine
More informationPROMAL2012 SOFTWARE PACKAGE A USER GUIDE
PROMAL2012 SOFTWARE PACKAGE A USER GUIDE 1. This manual is only for VISTA, WINDOWS 7 and WINDOWS 8 users. The PROMAL2012 software and manual are available at http://www.eng.usf.edu/~kaw/promal2012/ 2.
More informationInternational Journal of Advanced Engineering Technology EISSN
Research Article INTEGRATED FORCE METHOD FOR FIBER REINFORCED COMPOSITE PLATE BENDING PROBLEMS Doiphode G. S., Patodi S. C.* Address for Correspondence Assistant Professor, Applied Mechanics Department,
More informationAn integrated approach to the design of high performance carbon fibre reinforced risers  from micro to macro  scale
An integrated approach to the design of high performance carbon fibre reinforced risers  from micro to macro  scale Angelos Mintzas 1, Steve Hatton 1, Sarinova Simandjuntak 2, Andrew Little 2, Zhongyi
More informationFINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Ever J. Barbero Department of Mechanical and Aerospace Engineering West Virginia University USA CRC Press Taylor &.Francis Group Boca Raton London New York
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationOverview of Hygrothermally Stable Laminates with Improved Extensiontwist Coupling
Overview of Hygrothermally Stable Laminates with Improved Extensiontwist Coupling R. Haynes epartment of erospace Engineering, Georgia Institute of Technology 27 Ferst rive W, tlanta, G 33325, US robert.haynes@gatech.edu
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 36 Hygrothermal Stresses in Plates Lecture Overview Introduction Hygrothermal Strains Stiffness
More informationDynamic Responses of Composite Marine Propeller in Spatially Wake
Dynamic Responses of Composite Marine Propeller in Spatially Wake Dynamic Responses of Composite Marine Propeller in Spatially Wake Y. Hong a, X.D. He a,*, R.G. Wang a, Y.B. Li a, J.Z. Zhang a, H.M. Zhang
More informationDynamic analysis of Composite Micro Air Vehicles
Dynamic analysis of Composite Micro Air Vehicles Shishir Kr. Sahu Professor and Head, Civil Engineering, National Institute of Technology, Rourkela, India Email: sksahu@nitrkl.ac.in ABSTRACT The present
More informationThe effect of interfacial bonding on the damping behavior of nanocomposites
The effect of interfacial bonding on the damping behavior of nanocomposites Literature review The rapid and continuous growth in aerospace, automotive, and military applications requires special materials
More informationComposite Structural Mechanics using MATLAB
Session 2520 Composite Structural Mechanics using MATLAB Oscar Barton, Jr., Jacob B. Wallace United States Naval Academy Annapolis, Md 21402 Abstract In this paper MATLAB is adopted as the programming
More informationProbabilistic fatigue life prediction of multidirectional composite laminates
Composite Structures 69 () 9 www.elsevier.com/locate/compstruct Probabilistic fatigue life prediction of multidirectional composite laminates Yongming Liu, Sankaran Mahadevan * Department of Civil and
More informationSTUDY OF THE EFFECT OF COMPOSITE CONSTRAINED LAYERS IN VIBRATION DAMPING OF PLATES
Int. J. of Applied Mechanics and Engineering, 214, vol.19, No.1, pp.2329 DOI: 1.2478/ijame21415 Brief note STUDY OF THE EFFECT OF COMPOSITE CONSTRAINED LAYERS IN VIBRATION DAMPING OF PLATES K.S.K. SASIKUMAR
More informationFinite Element and Plate Theory Modeling of Acoustic Emission Waveforms. NASA Langley Research Center. Hampton, VA *University of Denver
Finite Element and Plate Theory Modeling of Acoustic Emission Waveforms W. H. Prosser, M. A. Hamstad + *, J. Gary +, and A. O Gallagher + NASA Langley Research Center Hampton, VA 236811 *University of
More informationDevelopment of a code to generate randomly distributed short fiber composites to estimate mechanical properties using FEM
International Journal of Theoretical and Applied Mechanics. ISSN 09736085 Volume 12, Number 4 (2017) pp. 863872 Research India Publications http://www.ripublication.com Development of a code to generate
More informationA RESEARCH ON NONLINEAR STABILITY AND FAILURE OF THIN WALLED COMPOSITE COLUMNS WITH OPEN CROSSSECTION
A RESEARCH ON NONLINEAR STABILITY AND FAILURE OF THIN WALLED COMPOSITE COLUMNS WITH OPEN CROSSSECTION H. Debski a*, J. Bienias b, P. Jakubczak b a Faculty of Mechanical Engineering, Department of Machine
More informationModelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations
Modelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations W. Van Paepegem *, I. De Baere and J. Degrieck Ghent
More informationLaminated Composite Plates and Shells
Jianqiao Ye Laminated Composite Plates and Shells 3D Modelling With 62 Figures Springer Table of Contents 1. Introduction to Composite Materials 1 1.1 Introduction 1 1.2 Classification of Composite Materials
More informationTrace a gamechanging discovery
Trace a gamechanging discovery Stephen W. Tsai Stanford University October 5, 2015 Topics Why trace? The one and only unifying constant Theory of trace simple; easy to understand CPly by Stanford/Chomarat
More informationEVALUATION OF THERMAL CYCLING INFLUENCE ON PEI/CARBON FIBER COMPOSITES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EVALUATION OF THERMAL CYCLING INFLUENCE ON PEI/CARBON FIBER COMPOSITES N.L. Batista 1, K. Iha 1, E.C. Botelho * 1 Department of Chemistry, Technological
More informationTensile Properties of ThermoplasticLaminated Composites Based on a Polypropylene Matrix Reinforced with Continuous Twaron Fibers
Tensile Properties of ThermoplasticLaminated Composites Based on a Polypropylene Matrix Reinforced with Continuous Twaron Fibers J. L. MENATUN, P. I. GONZALEZCHI Centro de Investigación Científica de
More informationModule6: Laminated CompositesII. Learning Unit1: M6.1. M 6.1 Structural Mechanics of Laminates
Module6: Laminated CompositesII Learning Unit1: M6.1 M 6.1 Structural Mechanics of Laminates Classical Lamination Theory: Laminate Stiffness Matrix To this point in the development of classical lamination
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationSTRUCTURAL EFFICIENCY VIA MINIMISATION OF ELASTIC ENERGY IN DAMAGE TOLERANT LAMINATES
ECCM1616 TH EUROPEAN CONFERENCE ON COMPOSITE MATERIALS, Seville, Spain, 2226 June 214 STRUCTURAL EFFICIENCY VIA MINIMISATION OF ELASTIC ENERGY IN DAMAGE TOLERANT LAMINATES M. Nielsen a, A. T. Rhead a,
More informationINTERNAL STRAIN MEASUREMENTS IN CFRP PLATES SUBJECTED TO IMPACT LOAD USING FBG SENSORS
INTERNAL STRAIN MEASUREMENTS IN CFRP PLATES SUBJECTED TO IMPACT LOAD USING FBG SENSORS J. Frieden, J. Cugnoni, J. Botsis, Th. Gmür, D. Coric Laboratoire de Mécanique appliquée et d Analyse de Fiabilité
More informationMODELING OF THE BEHAVIOR OF WOVEN LAMINATED COMPOSITES UNTIL RUPTURE
MODELING OF THE BEHAVIOR OF WOVEN LAMINATED COMPOSITES UNTIL RUPTURE Jean Paul Charles, Christian Hochard,3, Pierre Antoine Aubourg,3 Eurocopter, 375 Marignane cedex, France Unimeca, 6 rue J. Curie, 3453
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationPrediction of The Ultimate Strength of Composite Laminates Under InPlane Loading Using A Probabilistic Approach
Prediction of the Ultimate Strength of Composite Laminates Under InPlane Loading Prediction of The Ultimate Strength of Composite Laminates Under InPlane Loading Using A Probabilistic Approach Tae Jin
More informationPrediction of Elastic Constants on 3D Fourdirectional Braided
Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Liang Dao Zhou 1,2,* and Zhuo Zhuang 1 1 School of Aerospace,
More informationStrength Prediction Of Composite Laminate
Strength Prediction Of Composite te Prof. Yogananda. A 1, Mr. R. Vijayakumar 2 Assistant Professor, Department of Mechanical Engineering, East West Institute of Technology, Bangalore. Research Scholar,
More informationAmerican Society for Testing and Materials (ASTM) Standards. Mechanical Testing of Composites and their Constituents
Mechanical Testing of Composites and their Constituents American Society for Testing and Materials (ASTM) Standards Tests done to determine intrinsic material properties such as modulus and strength for
More informationOpenhole compressive strength prediction of CFRP composite laminates
Openhole compressive strength prediction of CFRP composite laminates O. İnal 1, A. Ataş 2,* 1 Department of Mechanical Engineering, Balikesir University, Balikesir, 10145, Turkey, inal@balikesir.edu.tr
More informationEffect of magnetostrictive material layer on the stress and deformation behaviour of laminated structure
IOP Conference Series: Materials Science and Engineering PAPER OPEN ACCESS Effect of magnetostrictive material layer on the stress and deformation behaviour of laminated structure To cite this article:
More informationNonlinear constitutive models for FRP composites using artificial neural networks
Mechanics of Materials 39 (2007) 1035 1042 www.elsevier.com/locate/mechmat Nonlinear constitutive models for FRP composites using artificial neural networks Rami HajAli *, HoanKee Kim School of Civil
More informationA STRUCTURE DESIGN OF CFRP REAR PRESSURE BULKHEAD WITHOUT STIFFENERS
Xi an, 225 th August 217 A STRUCTURE DESIGN OF CFRP REAR PRESSURE BULKHEAD WITHOUT STIFFENERS LI Zhongyang 1, LI Dong 2 Mailbox7235, Yanliang District, Xian, China, Email: zhongyangli@live.com Keywords:
More informationThe stiffness of plates
The stiffness of plates 1. Introduction The word plate is a collective term for elements in which forces can be transferred in two directions. Floors, walls, bridge slabs and laminates are all plates.
More information